QUT Digital Repository: http://eprints.qut.edu.au/
This is the author version published as: This is the accepted version of this article. To be published as :
This is the author version published as: Lynn, David Benjamin and Plagens, Owen and Castillo, Martin and Paulos, Todd and Steinberg, Ted (2010) The increased flammability of metallic materials burning in reduced gravity. In: 4th International Association for the Advancement of Space Safety Conference : Making Safety Matter, 1921 May 2010, Braun Center, Huntsville, Alabama. (Submitted (not yet accepted for publication))
Copyright 2010 [please consult the authors]
THE INCREASED FLAMMABILITY OF METALLIC MATERIALS BURNING IN REDUCED GRAVITY David Lynn(1), Owen Plagens(1), Martin Castillo(1), Todd Paulos (2) and Ted Steinberg(1) (1)
Queensland University of Technology, 2 George St, Brisbane QLD 4001, AUSTRALIA, Email: [email protected]
(2) Alejo Engineering Inc, 15562 Graham St, Huntington Beach, CA 92649, USA, Email: [email protected]
ABSTRACT Data generated in a normal gravity environment is often used in design and risk assessment for reduced gravity applications. It has been clearly demonstrated that this is a conservative approach for non-metallic materials which have been repeatedly shown to be less flammable in a reduced gravity environment. However, recent work has demonstrated this is not true for metallic materials. This work, conducted in a newly completed drop tower observed a significant increase in both lowest burn pressure and burn rate in reduced gravity. Hence the normal gravity qualification of a metallic materials’ lowest burn pressure or burn rate for reducedgravity or space-based systems is clearly not conservative. This paper presents a summary of this work and the results obtained for several metallic materials showing an increased flammability and burn rate for a range of oxygen pressures, and discusses the implications of this work on the fire-safety of spacebased systems. 1.
As demonstrated by the fire onboard the Mir space station , fires can and do occur in the space environment. The use of pressurised and/or concentrated oxygen or other oxidiser creates a very real fire hazard. When exposed to these oxidising environments, many metallic materials will burn quickly and violently if ignited. The isolated and critical nature of typical space systems means that the cost of any type of fire is very high in terms of personnel, economic and mission loss. In such environments, fire prevention by design is possible only by the application of accurate flammability knowledge. Metals flammability is measured by a standardised form of promoted ignition testing, in which the base of a test sample of specified dimensions is forcibly ignited. Testing is conducted in the upward burning configuration (in which the sample is ignited at its base and allowed to propagate up the rod if flammable) as results with greater repeatability are produced by this method. For a metal to be considered flammable under the test conditions, one of a specified number of tests must undergo independent burning, as evidenced by propagation further than a specified length (burn criteria). The burn criteria and number of tests may
vary dependent on the standard used, however the most commonly used standards are very similar. Tab. 1 shows the specific requirements of the ASTM and NASA standards. Table 1: ASTM and NASA standard requirements
Test Sample Dimensions
Φ3.2mm x 101.6mm
NASA  NASA-STD-(I)6001A Φ3.2mm x 101.6mm
Minimum Number of Tests
ASTM  G124-09 (2009)
Notes: 1. The ASTM standard recommends the use of the standard test sample; other configurations may be used. 2. The NASA standard requires the use of either the standard test sample (as stated) or a non-standard test sample of square crosssection with a side length of 3.2mm and minimum length of 101.6mm.
Two measurements are generated by this testing a) the lowest pressure at which a sample will support burning (this is recorded in the form of i) the Lowest Burn Pressure (LBP), and ii) the Highest No-Burn Pressure (HNBP)), and b) the Regression Rate of the Melting Interface (RRMI). The RRMI is the rate at which the sample is consumed, indicated by the propagation of the Solid-Liquid Interface (SLI), or the interface between the molten droplet at the base of the test sample and the remaining solid test sample. Typically the LBP/HNBP is used as a primary indicator of flammability, with the RRMI used to further define metals flammability. Previously it has been observed that under reduced gravity conditions, metals burn at an increased RRMI [4-7], and at lower pressures . Ward and Steinberg  explained the increase in RRMI by suggesting that more rapid heat transfer occurs in reduced gravity as a result of an increase in size of the SLI. Strong correlation between the increase in attachment area and increase in RRMI found in the subsequent investigations [7, 10] and microanalysis of quenched test samples showing a changed SLI in reduced gravity compared to normal gravity support this idea [11, 12]. Fig. 1 illustrates the difference in attachment geometry between normal and reduced gravity.
(~10-5g) low gravity. Detailed operating procedures and characteristics of the QUT drop tower are available elsewhere [13, 14]. Both normal and reduced gravity testing was conducted using the same combustion chamber to eliminate any experimental variations caused by the use of dissimilar chambers. 2.2. Ignition
Figure 1: Schematic showing comparative attachment geometry (SLI) for normal and reduced gravity  Further, Steinberg et al. [4, 5] hypothesised after early testing that metallic materials would exhibit a higher flammability in reduced gravity due to the absence of a growth and detachment cycle. This explanation seems highly probable and has been accepted by a number of researchers . Qualitative observations made in different reduced gravity studies suggest that higher temperatures may be reached within the molten droplet during burning in reduced gravity, supporting the idea of increased heat retention in reduced gravity. Lynn et al.  noted for several tests that during reduced gravity testing, a ‘considerable amount’ of molten metal was ejected from the molten droplet during burning, at a pressure at which the metal was found to be non-flammable in normal gravity. Steinberg et al.  observed a residue of chromium oxide on the inside of the combustion chamber after reduced gravity testing of 316 stainless steel. Both of these phenomena were concluded to be due to higher temperatures occurring within the burning droplet. This previous research suggests that the use of normal gravity information for reduced gravity use may or may not be appropriate. The objective of this work is to compare the flammability of commonly used engineering metallic materials under normal and reduced gravity, and utilising this information, examine whether the current testing methods are appropriate. 2.
2.1. Test Facilities and Apparatus All reduced gravity experiments were conducted using the Queensland University of Technology (QUT) Drop Tower, allowing approximately 2.0s of high quality
Test samples were ignited using aluminium-palladium igniter wire (tradename Pyrofuze®). The igniter wire was wrapped around a notch in the base of the sample (10 wraps) then attached to two chamber electrical feedthroughs. The igniter wire was resistively heated to initiate burning. When ignition occurs in normal gravity, the end of the test sample melts, and a molten droplet, including the igniter materials detaches from the base of the sample. In reduced gravity this drop detachment does not occur, and any ignition products used are retained as part of the molten droplet attached to the end of the rod. It has previously been suggested that when allowed to remain as part of the molten droplet, the igniter wire may act as a catalyst to the burning reaction . To avoid contamination of the molten droplet, the samples were ignited in normal gravity, the first droplet allowed to detach, and then the reduced gravity test commenced. 2.3. Materials In this study, 3.2mm diameter cylindrical test specimens were used to determine the flammability of two metallic alloys, Inconel® 718 (UNS N07718) and 316 stainless steel (UNS S31600). Tab. 2 details the exact chemical composition of the two alloys tested. Two sample lengths were used; 101.6mm (4 in.) in normal gravity, and 50.8mm (2 in.) in reduced gravity. The shorter samples were used in reduced gravity in order to ensure the burning aligned with the test chamber window through which a video recording was taken. Analytical modelling discussed in previous work  has shown that this difference in sample length has no effect on the ability of the sample to meet the burn criteria. The test medium used was commercially pure (3.0N, >99.9%) oxygen at pressures ranging between 2.24 MPa and 5.17 MPa.
Table 2: Chemical Composition of Test Alloys Material
Chemical Composition (wt%) Al